#------------------------------------------------------------------------------
#$Date: 2016-02-16 22:30:59 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/00/4340036.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4340036
loop_
_publ_author_name
'Meng, Chang-Yu'
'Chen, Hong'
'Wang, Peng'
_publ_section_title
;
 Syntheses, Structures, and Physical Properties of CsRE2Ag3Te5 (RE = Pr,
 Nd, Sm, Gd-Er) and RbRE2Ag3Te5 (RE = Sm, Gd-Dy).
;
_journal_issue                   13
_journal_name_full               'Inorganic chemistry'
_journal_page_first              6893
_journal_page_last               6903
_journal_paper_doi               10.1021/ic5007132
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety         'Ag1.20 Cs0.40 Gd0.80 Te2'
_chemical_formula_sum            'Ag1.2 Cs0.4 Gd0.8 Te2'
_chemical_formula_weight         563.61
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            10
_cell_length_a                   4.552(3)
_cell_length_b                   16.255(11)
_cell_length_c                   18.552(13)
_cell_measurement_reflns_used    791
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.4410
_cell_measurement_theta_min      2.7354
_cell_volume                     1372.7(16)
_computing_cell_refinement       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_collection       'CrystalClear (Rigaku Inc., 2007)'
_computing_data_reduction        'CrystalClear (Rigaku Inc., 2007)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 13.6612
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  SCXMini
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0337
_diffrn_reflns_av_sigmaI/netI    0.0223
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_number            5230
_diffrn_reflns_theta_full        27.43
_diffrn_reflns_theta_max         27.43
_diffrn_reflns_theta_min         2.51
_exptl_absorpt_coefficient_mu    26.712
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.6339
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            'silvery white'
_exptl_crystal_density_diffrn    6.819
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       chunk
_exptl_crystal_F_000             2336
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.09
_refine_diff_density_max         1.921
_refine_diff_density_min         -2.439
_refine_diff_density_rms         0.585
_refine_ls_extinction_coef       0.00010(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.336
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         904
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.336
_refine_ls_R_factor_all          0.0282
_refine_ls_R_factor_gt           0.0243
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0174P)²+79.4290P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0492
_refine_ls_wR_factor_ref         0.0754
_reflns_number_gt                864
_reflns_number_total             904
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5007132_si_002.cif
_cod_data_source_block           CsGd2Ag3Te5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4340029--4340040.cif.
;
_cod_original_cell_volume        1372.5(16)
_cod_original_sg_symbol_H-M      Cmcm
_cod_original_formula_sum        'Ag1.20 Cs0.40 Gd0.80 Te2'
_cod_database_code               4340036
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, -z+1/2'
'x, -y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z'
'-x, -y, -z'
'x, y, -z-1/2'
'x, -y, z-1/2'
'-x, y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, y+1/2, -z-1/2'
'x+1/2, -y+1/2, z-1/2'
'-x+1/2, y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cs Cs 0.0000 0.44149(8) 0.2500 0.0210(3) Uani 1 4 d S
Gd Gd 0.0000 0.30854(4) 0.59401(4) 0.0135(2) Uani 1 2 d S
Te1 Te 0.0000 0.93712(6) 0.61884(5) 0.0141(2) Uani 1 2 d S
Te2 Te 0.0000 0.32372(6) 0.07236(5) 0.0127(2) Uani 1 2 d S
Te3 Te 0.0000 0.75469(8) 0.2500 0.0146(3) Uani 1 4 d S
Ag1 Ag 0.0000 0.15863(12) 0.2500 0.0253(4) Uani 1 4 d S
Ag2 Ag 0.0000 0.91613(8) 0.03354(7) 0.0242(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Te3 Cs Te3 73.70(6) 5_445 5_545
Te3 Cs Te2 66.30(3) 5_445 .
Te3 Cs Te2 66.30(3) 5_545 .
Te3 Cs Te2 66.30(3) 5_445 10_556
Te3 Cs Te2 66.30(3) 5_545 10_556
Te2 Cs Te2 119.70(7) . 10_556
Te3 Cs Te1 139.49(3) 5_445 13_566
Te3 Cs Te1 93.17(4) 5_545 13_566
Te2 Cs Te1 143.07(2) . 13_566
Te2 Cs Te1 73.30(5) 10_556 13_566
Te3 Cs Te1 93.17(4) 5_445 6_464
Te3 Cs Te1 139.49(3) 5_545 6_464
Te2 Cs Te1 73.30(5) . 6_464
Te2 Cs Te1 143.07(2) 10_556 6_464
Te1 Cs Te1 118.73(6) 13_566 6_464
Te3 Cs Te1 93.17(4) 5_445 13_466
Te3 Cs Te1 139.49(3) 5_545 13_466
Te2 Cs Te1 143.07(2) . 13_466
Te2 Cs Te1 73.30(5) 10_556 13_466
Te1 Cs Te1 71.99(5) 13_566 13_466
Te1 Cs Te1 77.86(6) 6_464 13_466
Te3 Cs Te1 139.49(3) 5_445 6_564
Te3 Cs Te1 93.17(4) 5_545 6_564
Te2 Cs Te1 73.30(5) . 6_564
Te2 Cs Te1 143.07(2) 10_556 6_564
Te1 Cs Te1 77.86(6) 13_566 6_564
Te1 Cs Te1 71.99(5) 6_464 6_564
Te1 Cs Te1 118.73(6) 13_466 6_564
Te3 Cs Ag1 175.96(3) 5_445 5
Te3 Cs Ag1 110.34(6) 5_545 5
Te2 Cs Ag1 114.97(3) . 5
Te2 Cs Ag1 114.97(3) 10_556 5
Te1 Cs Ag1 41.69(3) 13_566 5
Te1 Cs Ag1 83.70(5) 6_464 5
Te1 Cs Ag1 83.70(5) 13_466 5
Te1 Cs Ag1 41.69(3) 6_564 5
Te3 Cs Ag1 110.34(6) 5_445 5_455
Te3 Cs Ag1 175.96(3) 5_545 5_455
Te2 Cs Ag1 114.97(3) . 5_455
Te2 Cs Ag1 114.97(3) 10_556 5_455
Te1 Cs Ag1 83.70(5) 13_566 5_455
Te1 Cs Ag1 41.69(3) 6_464 5_455
Te1 Cs Ag1 41.69(3) 13_466 5_455
Te1 Cs Ag1 83.70(5) 6_564 5_455
Ag1 Cs Ag1 65.63(6) 5 5_455
Te3 Cs Cs 126.85(3) 5_445 1_655
Te3 Cs Cs 53.15(3) 5_545 1_655
Te2 Cs Cs 90.0 . 1_655
Te2 Cs Cs 90.0 10_556 1_655
Te1 Cs Cs 54.00(3) 13_566 1_655
Te1 Cs Cs 126.00(3) 6_464 1_655
Te1 Cs Cs 126.00(3) 13_466 1_655
Te1 Cs Cs 54.00(3) 6_564 1_655
Ag1 Cs Cs 57.19(3) 5 1_655
Ag1 Cs Cs 122.81(3) 5_455 1_655
Te3 Cs Cs 53.15(3) 5_445 1_455
Te3 Cs Cs 126.85(3) 5_545 1_455
Te2 Cs Cs 90.0 . 1_455
Te2 Cs Cs 90.0 10_556 1_455
Te1 Cs Cs 126.00(3) 13_566 1_455
Te1 Cs Cs 54.00(3) 6_464 1_455
Te1 Cs Cs 54.00(3) 13_466 1_455
Te1 Cs Cs 126.00(3) 6_564 1_455
Ag1 Cs Cs 122.81(3) 5 1_455
Ag1 Cs Cs 57.19(3) 5_455 1_455
Cs Cs Cs 180.00(7) 1_655 1_455
Te3 Gd Te2 165.02(4) 9_566 10_556
Te3 Gd Te1 94.87(3) 9_566 5_545
Te2 Gd Te1 95.38(3) 10_556 5_545
Te3 Gd Te1 94.87(3) 9_566 5_445
Te2 Gd Te1 95.38(3) 10_556 5_445
Te1 Gd Te1 93.52(6) 5_545 5_445
Te3 Gd Te2 83.79(3) 9_566 6_455
Te2 Gd Te2 85.84(3) 10_556 6_455
Te1 Gd Te2 178.58(3) 5_545 6_455
Te1 Gd Te2 87.09(6) 5_445 6_455
Te3 Gd Te2 83.79(3) 9_566 6
Te2 Gd Te2 85.84(3) 10_556 6
Te1 Gd Te2 87.09(6) 5_545 6
Te1 Gd Te2 178.58(3) 5_445 6
Te2 Gd Te2 92.27(6) 6_455 6
Te3 Gd Ag2 139.18(3) 9_566 14_446
Te2 Gd Ag2 47.81(3) 10_556 14_446
Te1 Gd Ag2 103.00(5) 5_545 14_446
Te1 Gd Ag2 48.21(4) 5_445 14_446
Te2 Gd Ag2 78.36(5) 6_455 14_446
Te2 Gd Ag2 132.88(4) 6 14_446
Te3 Gd Ag2 139.18(3) 9_566 14_546
Te2 Gd Ag2 47.81(3) 10_556 14_546
Te1 Gd Ag2 48.21(4) 5_545 14_546
Te1 Gd Ag2 103.00(5) 5_445 14_546
Te2 Gd Ag2 132.88(4) 6_455 14_546
Te2 Gd Ag2 78.36(5) 6 14_546
Ag2 Gd Ag2 75.44(5) 14_446 14_546
Te3 Gd Ag1 46.76(4) 9_566 13_556
Te2 Gd Ag1 139.82(3) 10_556 13_556
Te1 Gd Ag1 48.98(3) 5_545 13_556
Te1 Gd Ag1 103.59(5) 5_445 13_556
Te2 Gd Ag1 129.63(4) 6_455 13_556
Te2 Gd Ag1 75.85(4) 6 13_556
Ag2 Gd Ag1 143.29(5) 14_446 13_556
Ag2 Gd Ag1 93.05(5) 14_546 13_556
Te3 Gd Ag1 46.76(4) 9_566 13_456
Te2 Gd Ag1 139.82(3) 10_556 13_456
Te1 Gd Ag1 103.59(5) 5_545 13_456
Te1 Gd Ag1 48.98(3) 5_445 13_456
Te2 Gd Ag1 75.85(4) 6_455 13_456
Te2 Gd Ag1 129.63(4) 6 13_456
Ag2 Gd Ag1 93.05(5) 14_446 13_456
Ag2 Gd Ag1 143.29(5) 14_546 13_456
Ag1 Gd Ag1 75.43(5) 13_556 13_456
Ag2 Te1 Ag2 63.32(6) 10_556 2_575
Ag2 Te1 Ag1 140.51(6) 10_556 9_566
Ag2 Te1 Ag1 156.17(5) 2_575 9_566
Ag2 Te1 Gd 76.90(3) 10_556 5_455
Ag2 Te1 Gd 118.42(4) 2_575 5_455
Ag1 Te1 Gd 76.33(4) 9_566 5_455
Ag2 Te1 Gd 76.90(3) 10_556 5
Ag2 Te1 Gd 118.42(4) 2_575 5
Ag1 Te1 Gd 76.33(4) 9_566 5
Gd Te1 Gd 93.52(6) 5_455 5
Ag2 Te1 Cs 133.23(3) 10_556 13_566
Ag2 Te1 Cs 85.57(5) 2_575 13_566
Ag1 Te1 Cs 75.24(5) 9_566 13_566
Gd Te1 Cs 149.51(4) 5_455 13_566
Gd Te1 Cs 90.31(5) 5 13_566
Ag2 Te1 Cs 133.23(3) 10_556 13_466
Ag2 Te1 Cs 85.57(5) 2_575 13_466
Ag1 Te1 Cs 75.24(5) 9_566 13_466
Gd Te1 Cs 90.31(5) 5_455 13_466
Gd Te1 Cs 149.51(4) 5 13_466
Cs Te1 Cs 71.99(5) 13_566 13_466
Ag2 Te2 Ag2 107.59(7) 5_545 5_445
Ag2 Te2 Gd 77.75(3) 5_545 10_556
Ag2 Te2 Gd 77.75(3) 5_445 10_556
Ag2 Te2 Gd 167.71(4) 5_545 6_454
Ag2 Te2 Gd 79.25(6) 5_445 6_454
Gd Te2 Gd 94.16(3) 10_556 6_454
Ag2 Te2 Gd 79.25(6) 5_545 6_554
Ag2 Te2 Gd 167.71(4) 5_445 6_554
Gd Te2 Gd 94.16(3) 10_556 6_554
Gd Te2 Gd 92.27(6) 6_454 6_554
Ag2 Te2 Cs 87.32(4) 5_545 .
Ag2 Te2 Cs 87.32(4) 5_445 .
Gd Te2 Cs 154.42(4) 10_556 .
Gd Te2 Cs 103.42(4) 6_454 .
Gd Te2 Cs 103.42(4) 6_554 .
Ag1 Te3 Ag1 111.09(9) 5_455 5
Ag1 Te3 Gd 79.08(3) 5_455 2_564
Ag1 Te3 Gd 79.08(3) 5 2_564
Ag1 Te3 Gd 79.08(3) 5_455 9_566
Ag1 Te3 Gd 79.08(3) 5 9_566
Gd Te3 Gd 140.89(6) 2_564 9_566
Ag1 Te3 Cs 161.31(5) 5_455 5
Ag1 Te3 Cs 87.61(6) 5 5
Gd Te3 Cs 105.54(3) 2_564 5
Gd Te3 Cs 105.54(3) 9_566 5
Ag1 Te3 Cs 87.61(6) 5_455 5_455
Ag1 Te3 Cs 161.31(5) 5 5_455
Gd Te3 Cs 105.54(3) 2_564 5_455
Gd Te3 Cs 105.54(3) 9_566 5_455
Cs Te3 Cs 73.70(6) 5 5_455
Te3 Ag1 Te3 111.09(9) 5_545 5_445
Te3 Ag1 Te1 107.75(3) 5_545 2_564
Te3 Ag1 Te1 107.75(3) 5_445 2_564
Te3 Ag1 Te1 107.75(3) 5_545 9_566
Te3 Ag1 Te1 107.75(3) 5_445 9_566
Te1 Ag1 Te1 114.79(9) 2_564 9_566
Te3 Ag1 Gd 54.16(3) 5_545 13_556
Te3 Ag1 Gd 115.04(5) 5_445 13_556
Te1 Ag1 Gd 137.11(4) 2_564 13_556
Te1 Ag1 Gd 54.69(4) 9_566 13_556
Te3 Ag1 Gd 115.04(5) 5_545 6_454
Te3 Ag1 Gd 54.16(3) 5_445 6_454
Te1 Ag1 Gd 54.69(4) 2_564 6_454
Te1 Ag1 Gd 137.11(4) 9_566 6_454
Gd Ag1 Gd 163.50(6) 13_556 6_454
Te3 Ag1 Gd 115.04(5) 5_545 13_456
Te3 Ag1 Gd 54.16(3) 5_445 13_456
Te1 Ag1 Gd 137.11(4) 2_564 13_456
Te1 Ag1 Gd 54.69(4) 9_566 13_456
Gd Ag1 Gd 75.43(5) 13_556 13_456
Gd Ag1 Gd 102.14(6) 6_454 13_456
Te3 Ag1 Gd 54.16(3) 5_545 6_554
Te3 Ag1 Gd 115.04(5) 5_445 6_554
Te1 Ag1 Gd 54.69(4) 2_564 6_554
Te1 Ag1 Gd 137.11(4) 9_566 6_554
Gd Ag1 Gd 102.14(6) 13_556 6_554
Gd Ag1 Gd 75.43(5) 6_454 6_554
Gd Ag1 Gd 163.50(6) 13_456 6_554
Te3 Ag1 Cs 157.27(5) 5_545 5_445
Te3 Ag1 Cs 91.64(6) 5_445 5_445
Te1 Ag1 Cs 63.07(4) 2_564 5_445
Te1 Ag1 Cs 63.07(4) 9_566 5_445
Gd Ag1 Cs 116.88(4) 13_556 5_445
Gd Ag1 Cs 77.82(3) 6_454 5_445
Gd Ag1 Cs 77.82(3) 13_456 5_445
Gd Ag1 Cs 116.88(4) 6_554 5_445
Te3 Ag1 Cs 91.64(6) 5_545 5_545
Te3 Ag1 Cs 157.27(5) 5_445 5_545
Te1 Ag1 Cs 63.07(4) 2_564 5_545
Te1 Ag1 Cs 63.07(4) 9_566 5_545
Gd Ag1 Cs 77.82(3) 13_556 5_545
Gd Ag1 Cs 116.88(4) 6_454 5_545
Gd Ag1 Cs 116.88(4) 13_456 5_545
Gd Ag1 Cs 77.82(3) 6_554 5_545
Cs Ag1 Cs 65.63(6) 5_445 5_545
Te2 Ag2 Te2 107.59(7) 5_455 5
Te2 Ag2 Te1 108.50(4) 5_455 10_556
Te2 Ag2 Te1 108.50(4) 5 10_556
Te2 Ag2 Te1 107.62(5) 5_455 2_574
Te2 Ag2 Te1 107.62(5) 5 2_574
Te1 Ag2 Te1 116.68(6) 10_556 2_574
Te2 Ag2 Ag2 126.20(4) 5_455 9_575
Te2 Ag2 Ag2 126.20(4) 5 9_575
Te1 Ag2 Ag2 58.59(5) 10_556 9_575
Te1 Ag2 Ag2 58.09(6) 2_574 9_575
Te2 Ag2 Gd 54.43(4) 5_455 14_456
Te2 Ag2 Gd 113.94(6) 5 14_456
Te1 Ag2 Gd 54.89(4) 10_556 14_456
Te1 Ag2 Gd 138.03(3) 2_574 14_456
Ag2 Ag2 Gd 99.42(6) 9_575 14_456
Te2 Ag2 Gd 113.94(6) 5_455 14_556
Te2 Ag2 Gd 54.43(4) 5 14_556
Te1 Ag2 Gd 54.89(4) 10_556 14_556
Te1 Ag2 Gd 138.03(3) 2_574 14_556
Ag2 Ag2 Gd 99.42(6) 9_575 14_556
Gd Ag2 Gd 75.44(5) 14_456 14_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Gd Te3 3.071(2) 9_566
Gd Te2 3.096(2) 10_556
Gd Te1 3.1240(17) 5_545
Gd Te1 3.1240(17) 5_445
Gd Te2 3.1564(17) 6_455
Gd Te2 3.1564(17) 6
Te1 Ag2 2.847(2) 10_556
Te1 Ag2 2.863(2) 2_575
Te1 Ag1 2.888(2) 9_566
Te1 Gd 3.1241(17) 5_455
Te1 Gd 3.1241(17) 5
Te2 Ag2 2.8204(17) 5_545
Te2 Ag2 2.8204(16) 5_445
Te2 Gd 3.096(2) 10_556
Te2 Gd 3.1564(17) 6_454
Te2 Gd 3.1564(17) 6_554
Te3 Ag1 2.7600(19) 5_455
Te3 Ag1 2.7600(19) 5
Te3 Gd 3.071(2) 2_564
Te3 Gd 3.071(2) 9_566
Ag1 Te3 2.7600(19) 5_545
Ag1 Te3 2.7600(19) 5_445
Ag1 Te1 2.888(2) 2_564
Ag1 Te1 2.888(2) 9_566
Ag1 Gd 3.7200(19) 13_556
Ag1 Gd 3.7200(19) 6_454
Ag1 Gd 3.7200(19) 13_456
Ag1 Gd 3.7200(19) 6_554
Ag2 Te2 2.8204(16) 5_455
Ag2 Te2 2.8204(16) 5
Ag2 Te1 2.847(2) 10_556
Ag2 Te1 2.863(2) 2_574
Ag2 Ag2 2.997(3) 9_575
